Refractory metals are a class of metals that are extraordinarily resistant to heat and wear. The expression is mostly used in the context of materials science, metallurgy and engineering. The definition of which elements belong to this group differs. The most common definition includes five elements: two of the fifth period (niobium and molybdenum) and three of the sixth period (tantalum, tungsten, and rhenium). They all share some properties, including a melting point above 2000 °C and high hardness at room temperature. They are chemically inert and have a relatively high density. Their high melting points make powder metallurgy the method of choice for fabricating components from these metals. Some of their applications include tools to work metals at high temperatures, wire filaments, casting molds, and chemical reaction vessels in corrosive environments. Partly due to the high melting point, refractory metals are stable against creep deformation to very high temperatures.
Most definitions of the term 'refractory metals' list the extraordinarily high melting point as a key requirement for inclusion. By one definition, a melting point above 4,000 °F (2,200 °C) is necessary to qualify. The five elements niobium, molybdenum, tantalum, tungsten and rhenium are included in all definitions, while the wider definition, including all elements with a melting point above 2,123 K (1,850 °C), includes a varying number of nine additional elements, titanium, vanadium, chromium, zirconium, hafnium, ruthenium, osmium and iridium. Transuranium elements (those above uranium, which are all unstable and not found naturally on earth) and technetium (melting point 2430 K or 2157 °C) are never considered to be part of the refractory metals.
|Melting point K||2750||2896||3290||3695||3459|
|Boiling point K||5017||4912||5731||5828||5869|
|Melting point °C||2477||2623||3017||3422||3186|
|Boiling point °C||4744||4639||5458||5555||5596|
|Young's modulus GPa||105||329||186||411||463|
|Vickers hardness MPa||1320||1530||873||3430||2450|
The melting point of the refractory metals are the highest for all elements except carbon, osmium and iridium. This high melting point defines most of their applications. All the metals are body-centered cubic except rhenium which is hexagonal close-packed. Most physical properties of the elements in this group vary significantly because they are members of different groups.
Creep resistance is a key property of the refractory metals. In metals, the starting of creep correlates with the melting point of the material; the creep in aluminium alloys starts at 200°C, while for refractory metals temperatures above 1500°C are necessary. This resistance against deformation at high temperatures makes the refractory metals suitable against strong forces at high temperature, for example in jet engines, or tools used during forging.
The refractory metals show a wide variety of chemical properties because they are members of three distinct groups in the periodic table. They are easily oxidized, but this reaction is slowed down in the bulk metal by the formation of stable oxide layers on the surface. Especially the oxide of rhenium is more volatile than the metal, and therefore at high temperature the stabilization against the attack of oxygen is lost, because the oxide layer evaporates. They all are relatively stable against acids.
Refractory metals are used in lighting, tools, lubricants, nuclear reaction control rods, as catalysts, and for their chemical or electrical properties. Because of their high melting point, refractory metal components are never fabricated by casting. The process of powder metallurgy is used. Powders of the pure metal are compacted, heated using electric current, and further fabricated by cold working with annealing steps. Refractory metals can be worked into wire, ingots, rebars, sheets or foil.
Molybdenum based alloys are widely used, because they are cheaper than superior tungsten alloys. The most widely used alloy of molybdenum is the Titanium-Zirconium-Molybdenum alloy TZM, composed of 0.5% titanium and 0.08% of zirconium (with molybdenum being the rest). The alloy exhibits a higher creep resistance and strength at high temperatures, making service temperatures of above 1060°C possible for the material. The high resistivity of Mo-30W an alloy of 70% molybdenum and 30 tungsten against the attack of molten zinc makes it the ideal material for casting zinc. It is also used to construct valves for molten zinc.
Molybdenum is the most commonly used of the refractory metals. Its most important use is as a strengthening alloy of steel. Structural tubing and piping often contains molybdenum, as do many stainless steels. Its strength at high temperatures, resistance to wear and low coefficient of friction are all properties which make it invaluable as an alloying compound. Its excellent anti-friction properties lead to its incorporation in greases and oils where reliability and performance are critical. Automotive constant-velocity joints use grease containing molybdenum. The compound sticks readily to metal and forms a very hard, friction resistant coating. Most of the world's molybdenum ore can be found in China, the USA, Chile and Canada.
Tungsten and its alloys
Up to 22% rhenium is alloyed with tungsten to improve its high temperature strength and corrosion resistance. Thorium as an alloying compound is used when electric arcs have to be established. The ignition is easier and the arc burns more stably than without the addition of thorium. For powder metallurgy applications, binders have to be used for the sintering process. For the production of the tungsten heavy alloy, binder mixtures of nickel and iron or nickel and copper are widely used. The tungsten content of the alloy is normally above 90%. The diffusion of the binder elements into the tungsten grains is low even at the sintering temperatures and therefore the interior of the grains is pure tungsten.
Tungsten and its alloys are often used in applications where high temperatures are present but still a high strength is necessary and the high density is not troublesome. Tungsten wire filaments provide the vast majority of household incandescent lighting, but are also common in industrial lighting as electrodes in arc lamps. Lamps get more efficient in the conversion of electric energy to light with higher temperatures and therefore a high melting point is essential for the application as filament in incandescent light. In the Gas tungsten arc welding (GTAW, also known as tungsten inert gas (TIG) welding) equipment uses a permanent, non-melting electrode. The high melting point and the wear resistance against the electric arc makes tungsten a suitable material for the electrode.
Tungsten's high density and strength is also a key property for its use in weapon projectiles, for example as an alternative to depleted Uranium for tank guns. Its high melting point makes tungsten a good material for applications like rocket nozzles, for example in the UGM-27 Polaris. Some of the applications of tungsten are not related to its refractory properties but simply to its density. For example, it is used in balance weights for planes and helicopters or for heads of golf clubs. In this applications similar dense materials like the more expensive osmium can also be used.
Niobium is nearly always found together with tantalum, and was named after Niobe, the daughter of the mythical Greek king Tantalus for whom tantalum was named. Niobium has many uses, some of which it shares with other refractory metals. It is unique in that it can be worked through annealing to achieve a wide range of strength and elasticity, and is the least dense of the refractory metals. It can also be found in electrolytic capacitors and in the most practical superconducting alloys. Niobium can be found in aircraft gas turbines, vacuum tubes and nuclear reactors.
An alloy used for liquid rocket thruster nozzles, such as in the main engine of the Apollo Lunar Modules, is C103, which consists of 89% niobium, 10% hafnium and 1% titanium. Another niobium alloy was used for the nozzle of the Apollo Service Module. As niobium is oxidized at temperatures above 400 °C, a protective coating is necessary for these applications to prevent the alloy from becoming brittle.
Tantalum and its alloys
Tantalum is one of the most corrosion resistant substances available.
Many important uses have been found for tantalum owing to this property, particularly in the medical and surgical fields, and also in harsh acidic environments. It is also used to make superior electrolytic capacitors. Tantalum films provide the second most capacitance per volume of any substance after Aerogel, and allow miniaturization of electronic components and circuitry. Many cellular phones and computers contain tantalum capacitors.
Rhenium is the most recently discovered refractory metal. It is found in low concentrations with many other metals, in the ores of other refractory metals, platinum or copper ores. It is useful as an alloy to other refractory metals, where it adds ductility and tensile strength. Rhenium alloys are being used in electronic components, gyroscopes and nuclear reactors. Rhenium finds its most important use as a catalyst. It is used as a catalyst in reactions such as alkylation, dealkylation, hydrogenation and oxidation. However its rarity makes it the most expensive of the refractory metals.
Advantages and shortfalls
Refractory metals and alloys attract the attention of investigators because of their remarkable properties and promising practical usefulness.
Physical properties of refractory metals, such as molybdenum, tantalum and tungsten, their strength, and high-temperature stability make them suitable material for hot metalworking applications and for vacuum furnace technology. Many special applications exploit these properties: for example, tungsten lamp filaments operate at temperatures up to 3073 K, and molybdenum furnace windings withstand to 2273 K.
However, poor low-temperature fabricability and extreme oxidability at high temperatures are shortcomings of most refractory metals. Interactions with the environment can significantly influence their high-temperature creep strength. Application of these metals requires a protective atmosphere or coating.
The refractory metal alloys of molybdenum, niobium, tantalum, and tungsten have been applied to space nuclear power systems. These systems were designed to operate at temperatures from 1350 K to approximately 1900 K. An environment must not interact with the material in question. Liquid alkali metals as the heat transfer fluids are used as well as the ultra-high vacuum.
The high-temperature creep strain of alloys must be limited for them to be used. The creep strain should not exceed 1–2%. An additional complication in studying creep behavior of the refractory metals is interactions with environment, which can significantly influence the creep behavior.
- "International Journal of Refractory Metals and Hard Materials". Elsevier. Retrieved 2010-02-07.
- Bauccio, Michael; American Society for Metals (1993). "Refractory metals". ASM metals reference book. ASM International. pp. 120–122. ISBN 978-0-87170-478-8.
- Metals, Behavior Of; Wilson, J. W (1965-06-01). "General Behaviour of Refractory Metals". Behavior and Properties of Refractory Metals. pp. 1–28. ISBN 978-0-8047-0162-4.
- Davis, Joseph R (2001). Alloying: understanding the basics. pp. 308–333. ISBN 978-0-87170-744-4.
- Borisenko, V. A. (1963). "Investigation of the temperature dependence of the hardness of molybdenum in the range of 20–2500°C". Soviet Powder Metallurgy and Metal Ceramics 1 (3): 182. doi:10.1007/BF00775076.
- Fathi, Habashi (2001). "Historical Introduction to Refractory Metals". Mineral Processing and Extractive Metallurgy Review 22 (1): 25–53. doi:10.1080/08827509808962488.
- Schmid, Kalpakjian (2006). "Creep". Manufacturing engineering and technology. Pearson Prentice Hall. pp. 86–93. ISBN 978-7-302-12535-8.
- Weroński, Andrzej; Hejwowski, Tadeusz (1991). "Creep-Resisting Materials". Thermal fatigue of metals. CRC Press. pp. 81–93. ISBN 978-0-8247-7726-5.
- Smallwood, Robert E. (1984). "TZM Moly Alloy". ASTM special technical publication 849: Refractory metals and their industrial applications: a symposium. ASTM International. p. 9. ISBN 978-0-8031-0203-3.
- Kozbagarova, G. A.; Musina, A. S.; Mikhaleva, V. A. (2003). "Corrosion Resistance of Molybdenum in Mercury". Protection of Metals 39 (4): 374–376. doi:10.1023/A:1024903616630.
- Gupta, C. K. (1992). "Electric and Electronic Industry". Extractive Metallurgy of Molybdenum. CRC Press. pp. 48–49. ISBN 978-0-8493-4758-0.
- Magyar, Michael J. "Commodity Summary 2009:Molybdenum" (PDF). United States Geological Survey. Retrieved 2010-04-01.
- Ervin, D.R.; Bourell, D.L.; Persad, C.; Rabenberg, L. (1988). "Structure and properties of high energy, high rate consolidated molybdenum alloy TZM". Materials Science and Engineering: A 102: 25. doi:10.1016/0025-5416(88)90529-0.
- Oleg D., Neikov (2009). "Properties of Molybdenum and Molybdenum Alloys powder". Handbook of Non-Ferrous Metal Powders: Technologies and Applications. Elsevier. pp. 464–466. ISBN 978-1-85617-422-0.
- Davis, Joseph R. (1997). "Refractory Metalls and Alloys". ASM specialty handbook: Heat-resistant materials. pp. 361–382. ISBN 978-0-87170-596-9.
- Lassner, Erik; Schubert, Wolf-Dieter (1999). Tungsten: properties, chemistry, technology of the element, alloys, and chemical compounds. Springer. pp. 255–282. ISBN 978-0-306-45053-2.
- National Research Council (U.S.), Panel on Tungsten, Committee on Technical Aspects of Critical and Strategic Material (1973). Trends in Usage of Tungsten: Report. National Research Council, National Academy of Sciences-National Academy of Engineering. pp. 1–3.
- Lassner, Erik; Schubert, Wolf-Dieter (1999). Tungsten: properties, chemistry, technology of the element, alloys, and chemical compounds. Springer. ISBN 978-0-306-45053-2.
- Harris, Michael K. (2002). "Welding Health and Safety". Welding health and safety: a field guide for OEHS professionals. AIHA. p. 28. ISBN 978-1-931504-28-7.
- Galvery, William L.; Marlow, Frank M. (2001). Welding essentials: questions & answers. Industrial Press Inc. p. 185. ISBN 978-0-8311-3151-7.
- Lanz, W.; Odermatt, W.; Weihrauch3, G. (7–11 May 2001). KINETIC ENERGY PROJECTILES: DEVELOPMENT HISTORY, STATE OF THE ART, TRENDS (PDF). 19th International Symposium of Ballistics. Interlaken, Switzerland.
- Ramakrishnan, P. (2007-01-01). "Powder metallurgyfor Aerospace Applications". Powder metallurgy : processing for automotive, electrical/electronic and engineering industry. New Age International. p. 38. ISBN 81-224-2030-3.
- Arora, Arran (2004). "Tungsten Heavy Alloy For Defence Applications". Materials Technology 19 (4): 210–216.
- Moxson, V. S.; (sam) Froes, F. H. (2001). "Fabricating sports equipment components via powder metallurgy". JOM 53 (4): 39. Bibcode:2001JOM....53d..39M. doi:10.1007/s11837-001-0147-z.
- Hebda, John (2001-05-02). "Niobium alloys and high Temperature Applications" (PDF). Niobium Science & Technology: Proceedings of the International Symposium Niobium 2001 (Orlando, Florida, USA) (Companhia Brasileira de Metalurgia e Mineração).
- Wilson, J. W. (1965). "Rhenium". Behavior and Properties of Refractory Metals. Stanford University Press. ISBN 978-0-8047-0162-4.
- Levitin, Valim (2006). High Temperature Strain of Metals and Alloys: Physical Fundamentals. WILEY-VCH. ISBN 978-3-527-31338-9.
- Brunner, T (2000). "Chemical and structural analyses of aerosol and fly-ash particles from fixed-bed biomass combustion plants by electron microscopy". 1st World Conference on Biomass for Energy and Industry: proceedings of the conference held in Sevilla, Spain, 5–9 June 2000 (London: James & James Ltd). ISBN 1-902916-15-8.
- Spink, Donald (1961). "Reactive Metals. Zirconium, Hafnium, and Titanium". Industrial & Engineering Chemistry 53 (2): 97–104. doi:10.1021/ie50614a019.
- Hayes, Earl (1961). "Chromium and Vanadium". Industrial & Engineering Chemistry 53 (2): 105–107. doi:10.1021/ie50614a020.